© Faculty of Mechanical Engineering, Belgrade. All rights
reserved FME Transactions (2009) 37, 61-70 61
Received: April 2009, Accepted: April 2009 Correspondence to: Dr
Friedrich Franek Vienna University of Technology, Institute of
Sensor and Actuator Systems Floragasse 7/2, A-1040 Wien, Austria
E-mail: [email protected]
Friedrich Franek University Professor, Deputy Head of
Department for Microsystem Technology Vienna University of
Institute of Sensor and Actuator Systems
Ewald Badisch Principal Scientist, Research Pool Leader
Austrian Center of Competence for Tribology – AC²T research
Martin Kirchgaßner General Manager
Castolin GesmbH, Vienna
Advanced Methods for Characterisation of Abrasion/Erosion
Resistance of Wear Protection Materials In many fields of industry,
abrasion and erosion processes are dominant wear mechanisms that
reduce lifetime of costly machine parts. Wear resistance against
abrasion and/or impact or the ability to withstand other complex
mechanical actions are often required. In order to quantify the
specific properties of material that are applied in such fields,
several test methods are in use. A certain discrepancy can be seen
between the systems approach and the aim to get information about
suitability of materials for practical applications simply from
specific material tests. This paper gives an overview over a
selection of relevant test equipment and procedures. In addition,
some examples are given for advanced studies on materials behaviour
combining tribological test, material analyses repectively
materialography, and mathematical methods in order to support – for
selected cases – the acquired correlation of materials properties
and wear resistance under severe conditions. Keywords: hardfacing
materials, abrasive wear, impact, test methods, morphology, wear
Abrasive wear  is a widely dominant wear mechanism especially
in a lot of industrial applications [2,3]. According to a “classic”
definition by SAE  abrasive wear concerns the removal of
material from a surface by mechanical action of abrasive (hard)
particles in contact with the surface. Arbitrary classifications of
abrasive wear are based on observed conditions :
Gouging Abrasion: The result of this type of abrasive wear is
the removal of large particles from a metal surface. Worn surfaces
show heavy gouges.
High Stress Grinding Abrasion: This type of abrasive wear occurs
during the progressive fragmentation or grinding of the abrasive
which was initially of small size and takes place on the surfaces
employed to grind the abrasive. The wear is believed to be caused
by concentrated compressive stress at the point of abrasive contact
and to result from plastic flowing and fatiguing of ductile
constituents and cracking of hard constituents of the metal
surface. The use of the words “high stress” in this classification
is intended to imply that the crushing strength of the abrasive is
Low Stress Scratching Abrasion or Erosion: The result of this
type of abrasive wear is scratching of the metal surface, and the
scratches are usually minute. The stress imposed on the abrasive
particle does not exceed the crushing strength of the abrasive.
Abrasive counterparts or particles are grooving the functional
surfaces of machine components or parts, like
tools, guidances, and raceways, under various tribological
interactions. Numerous basic operations to process raw materials,
among them crushing, classifying or conveying, are typical for
mining, steel and many other industries, and unavoidably related to
abrasion and different damaging effects due to abrasive particles,
like erosion, peening-like processes and also impacting. Core
components of converting plants such as crushers are exposed to
heavy wear and require efficient surface protection measures in
order to avoid costly downtimes and to reduce costs for expensive
spare parts . Both wear resistance against abrasion and/or
impact or the ability to withstand other complex mechanical actions
are often required to maintain the material’s structure and shape
of machine components and to extend the lifetime of machinery
equipment efficiently .
2. CONDITIONS FOR SPECIFIC TEST
Different wear mechanisms and the resulting wear amount show a
major influence on both the affected materials and the abrasive
matter, e.g. depending on the kinematic and kinetic properties of
abrasive particles, which is not surprising from a tribological
point of view.
Though the systems’ approach should govern the considerations of
wear behaviour a prevailing attitude can be observed in order to
characterise the applicability of materials for certain conditions
simply from material oriented tests. This is especially true for
the design and selection of hardfacing materials like iron-based
alloys that are to protect machinery equipment. The selection of
the most effective wear protection solution, especially in case of
combined wear, is either related to longterm practical experiences,
in situ tests or to applying alloys according to their hardness or
the content of specific hard phases such as tungsten carbide.
Simplified tests are feasible in terms of economic
62 ▪ VOL. 37, No 2, 2009 FME Transactions
restrictions and the need for statistically relevant results in
a reasonable time frame. Thus a number of test methods have been
introduced, more or less helpful for qualifying application
oriented material properties with regard to tribological
Yet it is unavoidable to study into detail the material
behaviour and the material structure being aware of the specific
stresses and wearing conditions that obviously vary according to
the concerned application each.
In spite of expectations that might arise from practical
engineering it is not seriously possible to characterize the
tribological performance of materials simply from a single test. In
order to evaluate the wear resistance under different fields of
operational demands, it is necessary to make use of several test
methods that not only provide abrasion but also other types of
tribological stresses. This means that also the combination of
stress variants have to be considered, which can be e.g.
combination of abrasion and impacts, or additional stressing
through high temperature. Another special condition could be due to
corrosive effects which may occur through different media (liquids,
Of course, different levels of tribological stresses that vary
have to be considered in the scope of this paper from “mild
abrasive wear” to heavy wearing conditions due to large abrasives
and/or high local stresses due to specific contact forces or
3. TEST METHODS FOR ABRASION/EROSION AND
3.1 Rotary platform double-head abrader
This type of setup is primarily used for tests under mild
abrasion conditions and commonly known as the TABER® Rotary
Platform Abraser . This “abrader” was already developed in the
1930’s in order to provide accelerated wear testing as it has been
used for research and development, quality and process control, and
generally for material evaluation. Several test procedures have
been introduced into industrial, national, and international
standards, e.g. [8-10]. The Taber Abraser generates a combination
of rolling and rubbing to cause wear to the tested material or
surface, respectively, being in contact with bonded abrasive
particles (Fig. 1).
Abrasives are applied in wearing rollers (abrading wheels) of
different composition (hard particles and binder). Test specimens
disks are spun on a turntable and are abraded by a pair of abrading
wheels for a specified number of cycles under a specified load. The
test method specifies that the change in haze of the test specimen
be determined as a measure of abrasion resistance. It is more
common, however, to see abrasion resistance reported as the change
in mass of the test specimen or change in mass per number of
cycles. Mass change is due to material loss from abrasion.
Thus wear is normally quantified as cumulative mass loss of the
plate mating against the wheels, or as a “Taber Wear Index” (mass
loss relating to 1000 cycles) typically after a test run of several
1000 cycles, with a typical test load (wheel load) of 10.2 N
(corresponding to a mass of 1000 g).
Figure 1. Rotary Platform Abraser: (a) test principle and (b)
test setup (acc. Taber® Industries )
Such type of abrasion tester is a versatile tool with many
regular test options as to type of wheel compositions. But it also
offers the opportunity to create specific combinations of test
samples, e.g. to invert the function of the samples, this means to
place the abrasives into the rotating base plate which then
produces wear of the counteracting wheels. Depending on the
abradant type and test specimen, the surface of the abrasive
component may change (becomes clogged) due to the transfer of
material from the test specimen to the abrading wheel, and thus
must be cleaned at frequent intervals or replaced. The test
conditions are comparatively mild due to the given level of load.
This may be the reason why this type of test – in spite of its
awareness level – is mainly used for testing of coatings and
different types of surface finishing.
3.2 Spherical abrasion test method
The spherical abrasion test method has beeen introduced as
Calowear® respectively Calotest (R) Tester by CSM Instruments SA
 as an instrument for a simple identification of coating
thickness but also to investigate the abrasive wear behaviours of
coated and uncoated materials.
The determination of the wear coefficient is carried out by the
wear crater technique. Thereby, a steel ball rolls over a sample
(in a special setup / CSM rig, Figs. 2a and b, or even on real
parts, Fig. 2c) with defined parameters, like rotation speed and
normal load, covered with an aqueous suspension of abrasive
material (silicon carbide or aluminium oxide powder). This ball
generates a spherical crater which will be sized with an optical
objective. These measured diameters correspond to the abrasive wear
3.3 Continuous abrasion test (CAT) – dry-sand
Abrasion tests with 3-body-abrasion condition under
comparatively low stress can be carried out according to ASTM G65
 on a dry-sand rubber-wheel tester (see Figure 2). Different
option or variants are used. Procedure A is a relatively severe
test which will rank metallic materials on a wide volume loss scale
FME Transactions VOL. 37, No 2, 2009 ▪ 63
to extreme abrasion resistance (Table 1). It is particularly
useful in ranking materials of medium to extreme abrasion
resistance. Procedure B is a short-term variation of Procedure A
for less resistant materials whereas Procedure C is a short-term
variation of Procedure A to be used for thin coatings.
Figure 2. Spherical abrasion test method: (a) and (b) CSM 
and (c) source: www.pvd-coatings.co.uk
Rotation speed and normal load are kept constant (for Procedure
A at 200 min-1 and 130 N respectively) over a sliding distance of
4309 m. Ottawa silica sand at grain size of 212 – 300 µm is used as
abrasive. Abrasion test results are reported as volume loss in
cubic millimetres (!) for the particular test procedure
Figure 3. Dry-sand wheel tester according ASTM G65
Table 1. Testing parameters used in HT-ET
Parameter Value Normal load 45 – 200 N
Disc diameter 229 mm (9 inches) Rotating speed 200 min-1
Relative velocity 2.4 m/s
Abrasive Silica sand (Ottawa type); 212 – 300 µm Feed rate of
abrasive 300 – 600 g/min
Size of samples 25 mm × 75 mm Test duration 40 min
Modifications of the G65 tests consider additional
features, e.g. to run the test specimen (especially
cemented carbides) in a wet slurry condition with a 6.65 inch
steel wheel according ASTM B-611 . Similarly, tests with the
slurry modification and special 7-inch rubber wheels can be
performed as described in ASTM G-105 . Such methods are
especially used to determine the resistance to abrasive wear of
ferrous materials for applications involving slurry abrasive media
(e.g. tilling soils and earth moving,) but can also be seen as
“Recommended Practice for Determining Resistance to Abrasive Wear
of ferrous metals using Rubber Wheel Abrasion Machine”, recommended
by the Society of Automotive Engineers .
3.4 High-temperature erosion test (HT-ET) – 2-body
Solid particle erosion tests can be performed in a centrifugal
four-channel accelerator  where up to 20 specimens can be
treated simultaneously under identical testing conditions (Fig. 4).
Examples of testing parameters are given in Table 2.
Figure 4. High temperature erosion test (HT-ET)
Table 2. Testing parameters used in HT-ET
Parameter Value Impact velocity 80 m/s Impact angles 30°,
Erodent Silica sand; 0.1 – 0.3 mm Total weight of erodent 6
Test temperatures RT, 300, 500, 650 °C The erosion rate is
determined as a volume loss of
the target sample per mass of abrasive particles hitting the
target (mm3/kg). An accuracy of 0.1 mg is obtained for the target
mass loss measurements. Each wear test is to be repeated three
For specific requirements investigation of steady state erosion
rate was made as a function of the impact angle at the abrasive
particle velocity of 80 m/s . The abrasive particles used in
this work were angular silica particles at a typical grain size of
0.1 – 0.3 mm. Erosion tests may be conducted at impact angles of
30° and 90°, respectively.
To study erosion at elevated temperature, the centrifugal
apparatus was put into the heated test chamber where tests at
enhanced temperatures were carried out at 300, 500 and 650 °C.
64 ▪ VOL. 37, No 2, 2009 FME Transactions
3.5 High-temperature continuous impact abrasion test (HT-CIAT) –
3-body impact abrasion
The HT-CIAT was developed at AC²T to determine the behaviour of
materials in continuous impact abrasive environment at elevated
temperatures [16,17]. Test principle is based on potential energy
which is cyclic turned into kinetic energy by free fall. The
samples are fixed in 45° and get continuously hit by the plunger,
while a constant abrasive flow is running between the sample and
the plunger as shown in Figure 5. The testing parameters are
summarized in Table 3. Impact energy, angle of impact and frequency
are chosen as 0.8 J, 45° and 2 Hz, respectively. The total number
of testing cycles is fixed to e.g. 7,200 which correlate to a
testing duration of 1 hour.
Figure 5. High temperature continuous impact abrasion test
Table 3. Testing parameters used in HT-CIAT
Parameter Value Impact energy 0.8 J Impact angle 45° Frequency 2
Testing cycles 7,200
Abrasive material Silica sand; 0.4 – 0.9 mm; angular Abrasive
flow 3 g/sec
Test temperature RT, 600 °C The abrasive material used for
typically silica sand of angular shape with a particle size of
0.4 – 0.9 mm. Typical flow rate is 3 g/sec. Experiments can be
carried out at room temperature but also at elevated temperatures
The plunger material used at these tests normally is a Co-rich
high speed steel.
Characterisation of wear behaviour is done by measuring the
weight loss of the samples (accuracy, 0.1 mg), by standard optical
microscopy (OM) and scanning electron microscopy (SEM). Also
cross-sections images of the worn specimen area have been made to
analyse the predominant mechanisms e.g. carbide breaking, cold work
hardening, composite layer formation and changes in the matrix
caused by high temperature.
3.6 Continuous impact abrasion test (CIAT) – 2-body impact
Wear tests on a specially designed impeller-tumbler apparatus
(CIAT) enable experimental simulation of combined impact and
abrasion. This testing device consists of a slowly rotating outer
tumbler and a fast rotating inner impeller at a rotation speed of
60 and 650 min-1, respectively, where the testing specimens are
mounted on [18-20]. The tumbler is filled with a defined amount of
abrasive, and is responsible for a controlled flow of abrasive
particles hitting the fast moving testing specimens (see Figure
Figure 6. Continuous impact abrasion tester (CIAT): (a) test
setup, (b) impeller-tumbler principle and (c) 1 – impeller with
samples to be tested and 2 – tumbler with filling (abrasive
Due to the kinematical situation the particles get in contact
with the specimen (surface exposed to abrasive particles, about 2.5
× 1.0 cm) at an impact velocity of approximately 10 m/s. As
abrasive for the experiments 1 kg of coarse corundum particles (5 –
10 mm) for high impact loading is used. In this case (depending on
the particle mass) a single particle impact energy of 28 mJ is
Typical duration of the runs is defined by 20 minutes. It is
recommended to repeat each test at least 3 times for statistic
calculation. The CIAT wear rate is calculated in volume loss
divided by testing time and mass of abrasive particles used. Wear
characterization is done by gravimetric mass loss of the testing
specimen during wear testing.
4. COMPLEMENTARY INVESTIGATIONS
4.1 Hardness mapping
Characterization of mechanical properties of materials and
especially of different phases and structural details
FME Transactions VOL. 37, No 2, 2009 ▪ 65
of materials can be done by hardness measurements. Those
investigations are typically carried out with a standard Vickers
hardness technique HV5 for macroscopic hardness. To determine
hardness of each phase in microstructure, e.g. hard particles and
metallic matrix, HV0.1 is used.
It is very useful to make use of an autosampling device which
provides multiple equidistant indents of a selected rectangular
4.2 Single impact test (SIT)
The utmost stress which can occur during
abrasion/erosion process is high energy impact of abrasive
particles. In order to study such single damaging events, wear
tests at high impact loading can be performed on a drop hammer
apparatus . The SIT was developed at AC²T to characterise the
impact resistance of materials against impacts with high energies
(up to 80 J). The test principle is based on potential energy
converted into kinetic energy by a free falling “hammer” of a total
mass m = 13.3 kg, which drops down very close to the edge of the
deposit material (see Figure 7).
Figure 7. Single impact tester (SIT) – drop hammer with conical
The sample is hit by the sharp edge of the hammer top of conical
shape (5° angle). Fall height of the hammer can be varied in a wide
range, so that the critical drop energy without breakout of the
edge can be detected for the different materials (alloys, welding
deposits, etc.) investigated. The impact leaves a dent on the
sample, which is firmly fixed so they cannot dodge during impact.
The samples’ deformation due to the impact is analysed, primarily
by quantifying the length (diameter) and depth of the indent. From
the latter the angle of the deformed area (impacted zone) can be
calculated which provides information about the relation between
elastic and plastic deformation of the material .
Fracture surface analysis should be carried out after drop
hammer testing in order to correlate the results with fracture
surface analysis, especially studying microstructure and
interfacial bonding behaviour of precipitations in metallic matrix
4.3 Single abrasion test (SAT) – scratch test
Whereas most of classical abrasion test methods are simulating a
multi-particle abrasion process where a high number of particles
are attacking the surface of a sample over a defined period of
time, in contrast to this the scratch-test method can be used to
simulate an ideal single-contact abrasion process. In general, a
very hard indenter (diamond) is used to simulate the contact
situation between a hard particle and a wearing surface in
application (example Figure 8). Such type of investigation can be
considered as generalisation of hardness testing.
Figure 8. 3D-image of the scratch mark, 50 µm-indenter, FN = 5
N, across differently hard phases
Based on this modelling situation, it can be assumed that the
deformation occurs in the counterpart material whereas on the
diamond indenter no significant deformation appears .
5. ADVANCED EVALUATION OF
ABRASION/EROSION RESISTANCE – EXAMPLES
5.1 Comparison of alloys under abrasion and impact
The main objective of this study  was to evaluate the wear
behaviour for pure abrasion and for combined wear of iron-based
alloys which are typically applied as hardfacing coatings by gas
metal arc welding. A crack free martensitic Fe-Cr-C alloy
containing finely precipitated Niobium carbides (A) was tested
against a conventional hypereutectic Fe-Cr-Nb-C alloy (B) already
well described in literature and thus a “reference material”.
Besides these lower alloyed materials on basis Fe-Cr-B-C
(hypoeutectic C; hypereutectic D) were set into comparison with a
new complex Fe-Cr-W-Mo-Nb alloy with high boron content (E) and a
synthetic multiphase alloy on iron base with around 50 wt. %
tungsten carbides (F), too. The microstructures of these materials
are shown in Figure 9.
CAT (3-body abrasion) tests were performed using ASTM G65
dry-sand rubber wheel tester (Procedure A). The comparison of the
materials’ behaviour both concerning their hardness (HV5) and their
abrasion resistance is shown in Figure 10.
High abrasive wear is observed for alloy A which is in good
agreement with the relative low hardness (see Figure 9). The lowest
abrasive wear resistance of the hardfacing alloys investigated was
observed for alloy C.
66 ▪ VOL. 37, No 2, 2009 FME Transactions
Figure 9. Microstructure of the investigated alloys
Figure 10. Abrasion behaviour and hardness – comparison of the 6
The influence of coarse primary precipitations on abrasive wear
resistance can be seen for alloys C and D, both alloys exhibiting
similar macroscopic hardness.
Also, continuous impact abrasion tests (CIAT) at different
impact levels were performed on the hardfacing alloy variants, some
results of which are depicted in Figure 11.
Figure 11. Abrasion behaviour (wear rate at low impact level,
fine-grained silica sand with 1.6. – 2.2 mm size) and hardness –
comparison of the 6 tested alloys
The lowest wear rates are obtained for alloys E and F. Alloy E
combines high density of carbo-borides with a very hard and tough
matrix. This microstructure is related to the complex composition,
to the high boron level, a sufficient content of carbide and boride
forming elements like Cr and V. It can be seen from the evaluation
that the testing parameters (i.e. the impact level) show a specific
influence on the results depending on the alloy structure .
5.2 Continuous impact abrasion test under different
This example gives an overview over a principle study 
comparing the wearing effects of five different kinds of abrasives
on samples of two different materials (Fe-based hardfacing alloys),
the main components of which are as follows:
• Alloy A (
FME Transactions VOL. 37, No 2, 2009 ▪ 67
micro-cracking of the hard phases gets prevailing resulting in
increased mass loss. For a single particle energy of higher than
8.26 mJ the embrittlement of hard phases is significant for the
progress of material loss. Highest mass loss can be observed at the
use of steel balls (see Figure 12).
Figure 12. Influence of the single particle impact energy on the
wear level of the tested alloys (low/high wear level)
It can be seen that for fine steel grit and fine quartz sand the
abrasive component is dominating, which means that the proportion
of abrasion is high compared to fatigue and impact. The load is too
low for significant fatigue and single impacts are not strong
enough for material separation.
The worn surface appears typical for rolling abrasive wear:
neither wear caused by micro-fracture of hard phases nor fatigue of
the matrix can be found at these low impacting energies caused by
steel grit and quartz sand.
5.3 Wear modelling of continuous impact abrasion
test at high impact loading
The single particle impact energy is assumed to be the main wear
relevant parameter for this type of tribological stress and is
therefore to be considered in the modelling of the deposited energy
in the material .
Based on the available energy rate for fracture initiation *bE
and a material related wear coefficient k the wear value W is given
by (1) to
*bEkW ⋅= . (1)
Furthermore, the deposited energy *dE is calculated
in (2) based on the kinetically deposited energy *kinE reduced
by the ratio which is dissipated by fracture of abrasives.
*kinI*d EnE ⋅⋅= ξ (2)
where ξ · n is the correction of the number of theoretical
impacts nI by the share of non broken particles. It is assumed that
the abrasive particles are hitting normal to the surface, whereas
no tangentially grooving movement of the particles occurs. The
material influence – which means the material specifically damaging
energy content – is considered by an apparent critical energy
density eCIAT [J/mm³]. This critical energy density includes a
plastic energy *plE , an elastic
rebound energy as well as an immediately fracture initiating
remaining energy *RE . Wear volume WV [mm3] can be calculated by
*V d CIAT/W E e= . (3)
Verification of the wear modelling has been done for a Fe-based
hardfacing alloy (
68 ▪ VOL. 37, No 2, 2009 FME Transactions
effects arising from carbide inter-particle distance surpass the
influence of carbide diameter and that of carbide fraction. Only
minor contribution to abrasive wear rates is related with matrix
hardness. Table 5. Composition properties and microstructure
parameters of the tested specimens
Coating Cr content WC
size [µm] Mean inter-particle
distance [µm] Type A high high ~ 130 291 Type B low high 100 357
Type C low high ~ 80 282 Type D low medium 63 241 Type E low low 63
Fundamental investigations on microstructures of
white cast iron have shown that resistance to abrasion is highly
influenced by carbide size and its inter-partic1e distance in
relation to the size of abrasives . More recent work of Doğan et
al.  pointed out that the role of inter-partic1e distance
between carbides is assessed more decisively than carbide size for
wear loss studies of materials.
The mean inter-particle distance LIPD was evaluated by
quantitative image analysis via Leica Qwin software applied on
images from fine polished and chemically etched samples according
IPD 3L L S= + ⋅ (4)
where L is the mean value of line distance distribution, and S
is the concerned standard deviation.
Abrasion tests on a dry-sand rubber-wheel tester according to
ASTM G65 procedure A were performed simulating conditions of
three-body abrasion under low stress (testing conditions:
rotational speed 200 min-1, normal load 130 N, sliding distance
4309 m; Ottawa silica sand, abrasive grain size 212 – 300 µm). For
statistical calculation each test was repeated three times. The
results are shown in Figure 14.
Figure 14. ASTM G65 (A) wear rates of the investigated Ni-based
A multiple regression analysis (by statistical data processing
tool Statgraphics, Statpoint Inc, USA) was used in order to
correlate abrasion relevant material parameters (carbide volume
fraction mean equivalent carbide diameter and LIPD) with low stress
wear rates. The functional form used for statistical modelling
linear in unknown coefficients, so that the model for the
response variable (wear rate) y could be set as follows
y β β x ε= + +∑ (5)
where βi stand for the unknown model coefficients, xi are
independent variables, n is the number of independent variables,
and ε is a random deviation respectively residual.
Three different parameter models were considered for the three
variables (area fraction, diameter and inter-particle distance).
For simplification of modelling these parameters were set
independent (though these variables are not independent!). The
parameter model based on carbide fraction shows with R2 = 95 %
(coefficient of determination) higher correlation than that based
on carbides’ diameter. Thus, wear resistance can be much more
addressed to carbide area fraction than to equivalent carbide
diameter (results corresponding with investigations reported in
literature ). Yet, the model based on inter-particle distance
shows superior fitting with R2 = 96 %.
Multiple regression analysis of different parameter models
enables better performance of the correlation. As it could be
shown, combining inter-particle distance and equivalent diameter as
independent variables delivers the best fitting model, with R2 = 99
%. The correlation of carbide inter-particle distance (LIPD) and
mean carbide diameter (D) with abrasive wear rate, respectively, is
shown on Figure 15. The inter-particle distance affects much more
the wear rate than the carbide diameter.
Figure 15. Microstructure parameters affecting the wear rate of
the tested Ni-based matrix systems: (a) inter-particle distance
LIPD and (b) mean carbide diameter D
FME Transactions VOL. 37, No 2, 2009 ▪ 69
6. CONCLUSION AND OUTLOOK
Characterisation of materials subject to abrasion/ erosion
processes conditions must be based on adequate experimental
methods. Such methods make use of various special tribometers; some
of them are commercially available. The tests have to be
accompanied by materialographic analyses. “Classical” methods
should be complemented by advanced modelling techniques and
mathematical tools that enable correlation of wear properties and
characteristic material properties for wear protection materials.
The latter will be studied extensively by novel investigation tools
providing both mechanical and structural material data.
Development and/or installation of the test equipment at AC²T
research GmbH as well as research work were partly funded from the
Austrian Kplus program (a governmental funding initiative for
precompetitive research for and with the industry).
 DIN 50 320 Wear: Terms, Systems Analysis of Wear processes,
Classification of the Field of Wear, German Standard, 1979.
 zum Gahr, K.-H.: Microstructure and Wear of Materials,
Elsevier, Amsterdam, 1987.
 Pamuk, U., Baydoğan, M., Nilüfer, B. and Çimenoğlu, H.: An
energetic approach to abrasive wear of a martensitic stainless
steel, Scripta Materialia, Vol. 42, No. 9, pp. 881-885, 2000.
 SAE J965 Abrasive Wear, Information Report, Society of
Automotive Engineers, Warrendale, 1966.
 Uetz, H.: Abrasion und Erosion, Carl Hanser Verlag, München,
 Weiß, H.: Verschleißverhalten von Mehrphasigen Werkstoffen
bei Mineralischem Verschleiß, MSc thesis, University of Applied
Sciences Wr. Neustadt, in cooperation with AC²T research, 2006.
 http://www.taberindustries.com/  CEN EN 14354 – Annex D
Test method for the
determination of the resistance to abrasion.  ASTM
F1978-00(2007)e2, Standard Test Method
for Measuring Abrasion Resistance of Metallic Thermal Spray
Coatings by Using the Taber Abraser, Annual Book of ASTM Standards,
Vol. 13.01, 2007.
 ISO 10074:1994 Specifications for Hard Anodic Oxidation
Coatings on Aluminum and its Alloys, 1994.
 CSM Products Catalogue – Advanced Mechanical Surface
Testing, CSM Instruments SA, Peseux, 2006.
 ASTM G65-04 Standard Test Method for Measuring Abrasion
Using the Dry Sand/Rubber Wheel Apparatus, Annual Book of ASTM
Standards, Vol. 03.02, 2004.
 ASTM B611-85(2005) Standard Test Method for Abrasive Wear
Resistance of Cemented Carbides,
Annual Book of ASTM Standards, Vol. 02.05, 2005.
 ASTM G105-02(2007) Standard Test Method for Conducting Wet
Sand/Rubber Wheel Abrasion Tests, Annual Book of ASTM Standards,
Vol. 03.02, 2007.
 Kulu, P., Hussainova, I. and Veinthal, R.: Solid particle
erosion of thermal sprayed coatings, Wear, Vol. 258, No. 1-4, pp.
 Badisch, E., Katsich, C., Winkelmann, H., Franek, F. and
Roy, M.: Wear behaviour of hardfaced Fe-Cr-C alloy and austenitic
steel under 2-body and 3-body conditions at elevated temperature,
in: Abstract Proceedings of the 2nd International Symposium
TriboCorrosion 2009, 17-18.03.2009, Wiener Neustadt, Austria.
 Badisch, E., Winkelmann, H. and Franek, F.:
High-temperature continuous impact abrasion testing (HAT-CIAT):
Wear behaviour of single and multiphase materials up to 750 °C,
prepared for: 18th International Baltic Conference on Engineering
Materials & Tribology – BALTMATTRIB 2009, 22-23.10.2009,
 Wilson, R.D. and Hawk, J.A.: Impeller wear impact-abrasive
wear test, Wear, Vol. 225-229, No. 2, pp. 1248-1257, 1999.
 Kirchgaßner, M., Badisch, E. and Franek, F.: Behaviour of
iron-based hardfacing alloys under abrasion and impact, Wear, Vol.
265, No. 5-6, pp. 772-779, 2008.
 Badisch, E., Kirchgaßner, M., Polak, R. and Franek, F.: The
comparison of wear properties of different Fe-based hardfacing
alloys in four kinds of testing methods, Tribotest, Vol. 14, No. 4,
pp. 225-233, 2008.
 Winkelmann, H., Varga, M., Badisch, E., Schweiger, H. and
Perko, J.: Blunting resistance of different cold work steels used
in the wood cutting industries, Wear, submitted for
 Krenn, S., Badisch, E. and Pauschitz, A.: Scratch test
method: energy dissipation and crack morphology, Proceedings of the
Institution of Mechanical Engineers, Part J: Journal of Engineering
Tribology, Vol. 222, No. 3, pp. 211-219, 2008.
 Badisch, E., Kirchgaßner, M. and Franek, F.: Continuous
impact/abrasion testing: influence of testing parameters on wear
behaviour, Proceedings of the Institution of Mechanical Engineers,
Part J: Journal of Engineering Tribology, accepted for
 Polak, R., Ilo, S. and Badisch, E.: Relation between
inter-particle distance (LIPD) and abrasion in multiphase
matrix-carbide materials, Tribology Letters, Vol. 33, No. 1, pp.
 Doğan, Ö.N., Hawk, J.A., Tylczak, J.H., Wilson, R.D. and
Govier, R.D.: Wear of titanium carbide reinforced metal matrix
composites, Wear, Vol. 225-229, No. 2, pp. 758-769, 1999.
70 ▪ VOL. 37, No 2, 2009 FME Transactions
НАПРЕДНЕ МЕТОДЕ ЗА ОДРЕЂИВАЊЕ
КАРАКТЕРИСТИКА МАТЕРИЈАЛА ОТПОРНИХ НА ХАБАЊЕ ПРИ АБРАЗИЈИ И
Фридрих Франек, Евалд Бадиш, Мартин Кирхгаснер
Абразија и ерозија су доминантни механизми хабања у многим
областима индустрије који скраћују радни век скупих машинских
делова. Отпорност на абразионо хабање или способност да се издрже
сложена механичка напрезања се често постављају као захтев. За
својстава материјала у наведеним областима користи се неколико
метода. Међу њима постоји одређена противречност у приступу и циљу
добијања информација, о томе колико су материјали погодни за
практичну употребу, само на основу одређених испитивања материјала.
Овај рад даје приказ избора релевантне опреме и поступака
испитивања. Осим тога, дато је неколико примера унапређених
испитивања понашања материјала, која представљају спој триболошких
испитивања, анализе материјала односно металографије и математичких
метода да би се, за одређене случајеве, пружили докази о добијеној
корелацији између својстава материјала и отпорности на хабање у
отежаним радним условима.